CASTING AND ITS TYPES
By WAQAS AHMED
Manufacturing is the production of goods for use or sale using
labor and machines, tools, chemical and biological processing, or
formulation. The term may refer to a range of human activity,
from handicraft to high tech, but is most commonly applied
to industrial production, in which raw materials are transformed
into finished goods on a large scale. Such finished goods may be
used for manufacturing other, more complex products, such
as aircraft, household appliances or automobiles,
There are many types of manufacturing process….
is a manufacturing process by which a
liquid material is usually poured into a mold,
which contains a hollow cavity of the desired
shape, and then allowed to solidify. The
solidified part is also known as a casting, which
is ejected or broken out of the mold to complete
Casting materials are usually metals or various cold
setting materials that cure after mixing two or more
components together; examples
are epoxy, concrete, plaster and clay. Casting is most
often used for making complex shapes that would be
otherwise difficult or uneconomical to make by other
Casting process can be divided into two basic
1. Those for which a new mold must be created for
casting (the expandable-mold processes)
2. Those that employ a permanent , reuseable mold ( the
Types of casting…!!!
are the basic types of casting..:
Shell mold casting
Permanent mold casting
Investment casting (lost wax casting)
of the expandable-mold processes begin
with some form of reuseable designs ………!!!
casting, a pattern is a replica of the object to
be cast, used to prepare the cavity into which
molten material will be poured during the
Patterns used in sand casting may be made of wood,
metal, plastics or other materials. Patterns are made to
exacting standards of construction, so that they can last
for a reasonable length of time, according to the quality
grade of the pattern being built, and so that they will
repeatably provide a dimensionally acceptable casting.
To produce cavities within the casting—such as
for liquid cooling in engine blocks and cylinder
heads—negative forms are used to produce cores
We shell discuss all types of casting one
Sand casting, also known as sand molded casting, is
a metal casting process characterized by using sand as
the mold material. The term "sand casting" can also refer
to an object produced via the sand casting process. Sand
castings are produced in
specialized factories called foundries. Over 70% of all
metal castings are produced via a sand casting process
Sand casting is relatively cheap and sufficiently refractory even for
steel foundry use. In addition to the sand, a suitable bonding agent
(usually clay) is mixed or occurs with the sand. The mixture is
moistened, typically with water, but sometimes with other
substances, to develop strength and plasticity of the clay and to
make the aggregate suitable for molding. The sand is typically
contained in a system of frames or mold boxes known as a flask.
The mold cavities and gate system are created by compacting the
sand around models, or patterns, or carved directly into the sand.
There are six steps in this process:
1. Place a pattern in sand to create a mold.
2. Incorporate the pattern and sand in a gating system.
3. Remove the pattern.
4. Fill the mold cavity with molten metal.
5. Allow the metal to cool.
6. Break away the sand mold and remove the casting
Die casting is a metal casting process that is characterized by
forcing molten metal under high pressure into a mold cavity. The mold
cavity is created using two hardened tool steel dies which have been
machined into shape and work similarly to an injection mold during the
process. Most die castings are made from non-ferrous metals,
specifically zinc, copper, aluminium, magnesium, lead, pewter and tin
based alloys Depending on the type of metal being cast, a hot- or coldchamber machine is used.
The casting equipment and the metal dies represent large capital costs
and this tends to limit the process to high volume production.
Manufacture of parts using die casting is relatively simple, involving
only four main steps, which keeps the incremental cost per item low. It
is especially suited for a large quantity of small to medium sized
castings, which is why die casting produces more castings than any
other casting process. Die castings are characterized by a very
good surface finish (by casting standards) and dimensional consistency
The main die casting alloys are: zinc, aluminium, magnesium, copper, lead, & tin;
although uncommon, ferous
The following is a summary of the advantages of each alloy:
Zinc: the easiest metal to cast; high ductility; high impact strength; easily plated; economical
for small parts; promotes long die life.
Aluminium: lightweight; high dimensional stability for complex shapes and thin walls;
good corrosion resistance; good mechanical properties; high thermal and electrical conductivity;
retains strength at high temperatures.
Magnesium: the easiest metal to machine; excellent strength-to-weight ratio; lightest
alloy commonly die cast.
Copper: high hardness; high corrosion resistance; highest mechanical properties of alloys
die cast; excellent wear resistance; excellent dimensional stability; strength approaching that of
Lead and tin: high density; extremely close dimensional accuracy; used for special forms
of corrosion resistance. Such alloys are not used in foodservice applications for public
health reasons. Type metal, an alloy of Lead, Tin and Antimony (with sometimes traces of
Copper) is used for casting hand set type in letterpress printing and hot foil blocking.
There are two basic types of die casting machines:
hot-chamber machines & cold-chamber machines.
These are rated by how much clamping force they can
apply. Typical ratings are between 400 and 4,000 st
(2,500 and 25,000 kg)
Hot-chamber machines, also known as gooseneck machines, rely
upon a pool of molten metal to feed the die. At the beginning of the
cycle the piston of the machine is retracted, which allows the molten
metal to fill the "gooseneck". The pneumatic or hydraulic powered
piston then forces this metal out of the gooseneck into the die. The
advantages of this system include fast cycle times (approximately 15
cycles a minute) and the convenience of melting the metal in the
casting machine. The disadvantages of this system are that highmelting point metals cannot be utilized and aluminium cannot be
used because it picks up some of the iron while in the molten pool.
Due to this, hot-chamber machines are primarily used with zinc, tin,
and lead based alloys
These are used when the casting alloy cannot be used in hotchamber machines; these include aluminium, zinc alloys with a large
composition of aluminium, magnesium and copper. The process for
these machines start with melting the metal in a separate
furnace. Then a precise amount of molten metal is transported to the
cold-chamber machine where it is fed into an unheated shot chamber
(or injection cylinder). This shot is then driven into the die by a
hydraulic or mechanical piston. This biggest disadvantage of this
system is the slower cycle time due to the need to transfer the molten
metal from the furnace to the cold-chamber machine
Two dies are used in die casting; one is called the "cover die half"
and the other the "ejector die half". Where they meet is called the
parting line. The cover die contains the sprue (for hot-chamber
machines) or shot hole (for cold-chamber machines), which allows
the molten metal to flow into the dies; this feature matches up with
the injector nozzle on the hot-chamber machines or the shot chamber
in the cold-chamber machines. The ejector die contains the ejector
pins and usually the runner, which is the path from the sprue or shot
hole to the mold cavity. The cover die is secured to the stationary, or
front , platen of the casting machine, while the ejector die is attached
to the movable platen. The mold cavity is cut into two cavity inserts,
which are separate pieces that can be replaced relatively easily and
bolt into the die halves
The following are the four steps in traditional die
casting, also known as high-pressure die casting,
these are also the basis for any of the die casting
Advantages of die casting:
Excellent dimensional accuracy (dependent on casting material, but typically 0.1 mm
for the first 2.5 cm (0.005 inch for the first inch) and 0.02 mm for each additional
centimeter (0.002 inch for each additional inch).
Smooth cast surfaces (Ra 1–2.5 micrometres or 0.04–0.10 thou ).
Reduces or eliminates secondary machining operations.
Rapid production rates.
Casting of low fluidity metals.
The main disadvantage to die casting is the very high capital cost. Both
the casting equipment required and the dies and related components are very
costly, as compared to most other casting processes. Therefore to make die
casting an economic process a large production volume is needed. Other
disadvantages are that the process is limited to high-fluidity metals, and
casting weights must be between 30 grams (1 oz) and 10 kg (20 lb). In the
standard die casting process the final casting will have a small amount of
porosity. This prevents any heat treating or welding, because the heat causes
the gas in the pores to expand, which causes micro-cracks inside the part
and exfoliation of the surface
Shell molding, also known as shell-mold casting, is an expendable
mold casting process that uses a resin covered sand to form
As compared to sand casting, this process has better dimensional accuracy, a
higher productivity rate, and lower labor requirements. It is used for small to
medium parts that require high precision. Shell mold casting is a metal
casting process similar to sand casting, in that molten metal is poured into an
expendable mold. However, in shell mold casting, the mold is a thin-walled
shell created from applying a sand-resin mixture around a pattern. The
pattern, a metal piece in the shape of the desired part, is reused to form
multiple shell molds. A reusable pattern allows for higher production rates,
while the disposable molds enable complex geometries to be cast. Shell mold
casting requires the use of a metal pattern, oven, sand-resin mixture, dump
box, and molten metal.
Shell mold casting allows the use of both ferrous and non-ferrous metals,
most commonly using cast iron, carbon steel, alloy steel, stainless steel,
aluminum alloys, & copper alloys. Typical parts are small-to-medium in
size and require high accuracy, such as gear housings, cylinder heads,
connecting rods, & lever arms
shell mold casting process consists of
the following steps:
Examples of shell molded items include gear housings, cylinder
heads & connecting rods. It is also used to make high-precision
The process of creating a shell mold consists of six steps:
Fine silica sand that is covered in a thin (3–6%) thermosetting phenolic
resin and liquid catalyst is dumped, blown, or shot onto a hot pattern. The
pattern is usually made from cast iron and is heated to 230 to 315 C (450 to
600 F). The sand is allowed to sit on the pattern for a few minutes to allow
the sand to partially cure.
The pattern and sand are then inverted so the excess sand drops free of the
pattern, leaving just the "shell". Depending on the time and temperature of
the pattern the thickness of the shell is 10 to 20 mm (0.4 to 0.8 in).
The pattern and shell together are placed in an oven to finish curing the
sand. The shell now has a tensile strength of 350 to 450 psi
(2.4 to 3.1 MPa).
The hardened shell is then stripped from the pattern.
Two or more shells are then combined, via clamping or gluing using a
thermoset adhesive, to form a mold. This finished mold can then be used
immediately or stored almost indefinitely.
For casting the shell mold is placed inside a flask and surrounded with shot,
sand, or gravel to reinforce the shell.
The machine that is used for this process is called a shell molding machine. It heats
the pattern, applies the sand mixture, and bakes the shell.
One of the greatest advantages of this process is that it can be
completely automated for mass production. The high productivity,
low labor costs, good surface finishes, and precision of the process
can more than pay for itself if it reduces machining costs
. There are also few problems due to gases, because of the absence
of moisture in the shell, and the little gas that is still present easily
escapes through the thin shell. When the metal is poured some of the
resin binder burns out on the surface of the shell, which makes
shaking out easy.
Permanent mold casting is metal casting process that employs
reusable molds ("permanent molds"), usually made from metal. The
most common process uses gravity to fill the mold, however gas
pressure or a vacuum are also used. A variation on the typical gravity
casting process, called slush casting, produces hollow castings.
Common casting metals are aluminum, magnesium,
and copper alloys. Other materials include tin, zinc, and lead alloys
and iron and steel are also cast in graphite molds
There are four main types of permanent mold casting:
The gravity process begins by preheating the mold to 150200 C (300-400 F) to ease the flow and reduce thermal
damage to the casting. The mold cavity is then coated with
a refractory material or a mold wash, which prevents the
casting from sticking to the mold and prolongs the mold life.
Any sand or metal cores are then installed and the mold is
clamped shut. Molten metal is then poured into the mold.
Soon after solidification the mold is opened and the casting
removed to reduce chances of hot tears. The process is then
started all over again, but preheating is not required because
the heat from the previous casting is adequate and the
refractory coating should last several castings. Because this
process is usually carried out on large production run
workpieces automated equipment is used to coat the mold,
pour the metal, and remove the casting
Slush casting is a variant of permanent molding casting
to create a hollow casting or hollow cast. In the process
the material is poured into the mold and allowed to cool
until a shell of material forms in the mold. The remaining
liquid is then poured out to leave a hollow shell. The
resulting casting has good surface detail but the wall
thickness can vary. The process is usually used to
cast ornamental products, such
as candlesticks, lamp bases, and statuary, from lowmelting-point materials. A similar technique is used to
make hollow chocolate figures
for Easter and Christmas
Low-pressure permanent mold (LPPM) casting uses a
gas at low pressure, usually between 3 and 15 psig (20 to
100 kPag) to push the molten metal into the mold cavity.
The pressure is applied to the top of the pool of liquid,
which forces the molten metal up a refractory pouring
tube and finally into the bottom of the mold. The pouring
tube extends to the bottom of the ladle so that the
material being pushed into the mold is exceptionally
clean. No risers are required because the applied pressure
forces molten metal in to compensate for shrinkage.
Yields are usually greater than 85% because there is no
riser and any metal in the pouring tube just falls back
into the ladle for reuse
Vacuum permanent mold casting retains all of the
advantages of LPPM casting, plus the dissolved gases in
the molten metal are minimized and molten metal
cleanliness is even better. The process can handle thinwalled profiles and gives an excellent surface finish.
Mechanical properties are usually 10 to 15% better than
gravity permanent mold castings. The process is limited
in weight to 0.2 to 5 kg
The main advantages are the reusable mold, good
surface finish,&good dimensional accuracy
There are three main disadvantages:
high tooling cost,
limited to low-melting-point metals,
short mold life
Investment casting is an industrial process based on and
also called lost-wax casting, one of the oldest known
metal-forming techniques .From 5,000 years ago, when
bees wax formed the pattern, to today’s high-technology
waxes, refractory materials and specialist alloys, the
castings allow the production of components with
accuracy, repeatability, versatility and integrity in a
variety of metals and high-performance alloys.
The process is generally used for small castings, but has been used to
produce complete aircraft door frames, steel castings of up to 300 kg
(660 lbs) and aluminium castings of up to 30 kg (66 lbs). It is
generally more expensive per unit than die casting or sand casting, but
has lower equipment costs. It can produce complicated shapes that
would be difficult or impossible with die casting, yet like that process, it
requires little surface finishing and only minor machining..
Produce a master pattern:
Produce the wax patterns:
Assemble the wax patterns:
Burnout & preheating:
a master pattern:
An artist or mould-maker creates an original pattern
from wax, clay, wood, plastic, steel, or another material….!!!
A mould, known as the master die, is made of the master
pattern. The master pattern may be made from a lowmelting-point metal, steel, or wood. If a steel pattern was
created then a low-melting-point metal may be cast
directly from the master pattern. Rubber moulds can also
be cast directly from the master pattern. The first step
may also be skipped if the master die is machined
directly into steel.
the wax patterns:
Although called a wax pattern, pattern materials also include plastic
and frozen mercury. Wax patterns may be produced in one of two
ways. In one process the wax is poured into the mold and swished
around until an even coating, usually about 3 mm (0.12 in) thick,
covers the inner surface of the mould. This is repeated until the
desired thickness is reached. Another method is filling the entire
mould with molten wax, and let it cool, until a desired thickness has
set on the surface of the mould. After this the rest of the wax is
poured out again, the mould is turned upside down and the wax
layer is left to cool and harden. With this method it is more difficult
to control the overall thickness of the wax layer
the wax patterns:
The wax pattern is then removed from the mould. Depending on the
application multiple wax patterns may be created so that they can all
be cast at once. In other applications, multiple different wax patterns
may be created and then assembled into one complex pattern. In the
first case the multiple patterns are attached to a wax sprue, with the
result known as a pattern cluster, or tree; as many as several
hundred patterns may be assembled into a tree. Foundries often use
registration marks to indicate exactly where they go. The wax
patterns are attached to the sprue or each other by means of a heated
metal tool. The wax pattern may also be chased, which means
the parting line or flashing are rubbed out using the heated metal
tool. Finally it is dressed, which means any other imperfections are
addressed so that the wax now looks like the finished piece.
The ceramic mould, known as the investment, is produced by three
repeating steps: coating, stuccoing, and hardening. The first step
involves dipping the cluster into a slurry of fine refractory material
and then letting any excess drain off, so a uniform surface is
produced. This fine material is used first to give a smooth surface
finish and reproduce fine details. In the second step, the cluster
is stuccoed with a coarse ceramic particle, by dipping it into
a fluidised bed, placing it in a rainfall-sander, or by applying by
hand. Finally, the coating is allowed to harden. These steps are
repeated until the investment is the required thickness, which is
usually 5 to 15 mm
The investment is then allowed to completely dry, which can take 16
to 48 hours. Drying can be enhanced by applying a vacuum or
minimizing the environmental humidity. It is then turned upsidedown and placed in a furnace or autoclave to melt out and/or
vaporize the wax. Most shell failures occur at this point because the
waxes used have a thermal expansion coefficient that is much
greater than the investment material surrounding it, so as the wax is
heated it expands and induces great stresses. In order to minimize
these stresses the wax is heated as rapidly as possible so that the
surface of the wax can melt into the surface of the investment or run
out of the mold, which makes room for the rest of the wax to
expand. In certain situations holes may be drilled into the mold
beforehand to help reduce these stresses. Any wax that runs out of
the mold is usually recovered and reused.
The mold is then subjected to a burnout, which heats the mold
between 870 C & 1095 C to remove any moisture and residual
wax, and to sinter the mold. Sometimes this heating is also used as
the preheat, but other times the mold is allowed to cool so that it can
be tested. If any cracks are found they can be repaired with ceramic
slurry or special cements. The mold is preheated to allow the metal
to stay liquid longer to fill any details and to increase dimensional
accuracy, because the mold and casting cool together
The investment mold is then placed cup-upwards into a tub filled
with sand. The metal may be gravity poured, but if there are thin
sections in the mold it may be filled by applying positive air
pressure, vacuum cast, tilt cast, pressure assisted pouring,
or centrifugal cast
The shell is hammered, media blasted, vibrated, waterjeted, or
chemically dissolved (sometimes with liquid nitrogen) to release the
casting. The sprue is cut off and recycled. The casting may then be
cleaned up to remove signs of the casting process, usually
The investment shell for casting a turbocharger rotor:
A view of the interior investment shows the smooth
surface finish and high level of detail:
of Investment casting:
A very smooth surface is obtained with no parting line.
Dimensional accuracy is good.
Certain unmachinable parts can be cast to preplanned
of Investment casting:
This process is expensive, is usually limited to small
casting, and presents some difficulties where cores are
Holes cannot be smaller than 1/16 in. (1.6mm) and
should be no deeper than about 1.5 times the diameter.
Investment castings require very long production-cycle
times versus other casting processes.
This process is practically infeasible for high-volume
manufacturing, due to its high cost and long cycle times.
Investment casting is used in the aerospace and power
generation industries to produce turbine blades with
complex shapes or cooling systems
Lost-foam casting (LFC) is a type of evaporativepattern casting process that is similar to investment
casting except foam is used for the pattern instead
This process takes advantage of the low boiling point of
foam to simplify the investment casting process by
removing the need to melt the wax out of the mold
First, a pattern is made from polystyrene foam, which can be done many different ways.
For small volume runs the pattern can be hand cut or machined from a solid block of foam;
if the geometry is simple enough it can even be cut using a hot-wire foam cutter. If the
volume is large, then the pattern can be mass-produced by a process similar to injection
molding. Pre-expanded beads of polystyrene are injected into a preheated
aluminum mold at low pressure. Steam is then applied to the polystyrene which causes it to
expand more to fill the die. The final pattern is approximately 97.5% air and 2.5%
polystyrene. Pre-made pouring basins, runners, and risers can be hot glued to the pattern to
Next, the foam cluster is coated with ceramic investment, also known as
the refractory coating, via dipping, brushing, spraying or flow coating. This coating creates
a barrier between the smooth foam surface and the coarse sand surface. Secondly it
controls permeability, which allows the gas created by the vaporized foam pattern to
escape through the coating and into the sand. Controlling permeability is a crucial step to
avoid sand erosion. Finally, it forms a barrier so that molten metal does not penetrate or
cause sand erosion during pouring. After the coating dries, the cluster is placed into a flask
and backed up with un-bonded sand. The sand is then compacted using a vibration table.
Once compacted, the mold is ready to be poured . Automatic pouring is commonly used in
LFC, as the pouring process is significantly more critical than in conventional foundry
There is no bake-out phase, as for lost-wax. The melt is poured directly into the foam-filled
mould, burning out the foam as it pours. As the foam is of low density, the waste gas
produced by this is relatively small and can escape through mould permeability, as for the
usual out gassing control
This casting process is advantageous for very complex
castings that would regularly require cores. It is also
dimensionally accurate, maintains an excellent surface finish,
requires no draft, and has no parting lines so no flash is
formed. As compared to investment casting, it is cheaper
because it is a simpler process and the foam is cheaper than
the wax. Risers are not usually required due to the nature of
the process; because the molten metal vaporizes the foam the
first metal into the mold cools more quickly than the rest,
which results in natural directional solidificationFoam is easy
to manipulate, carve and glue, due to its unique properties
The two main disadvantages are that pattern costs can be high
for low volume applications and the patterns are easily
damaged or distorted due to their low strength.
If a die is used to create the patterns there is a large initial
Centrifugal casting or roto-casting is
a casting technique that is typically used to cast thinwalled cylinders. It is noted for the high quality of the
results attainable, particularly for precise control of their
metallurgy and crystal structure. Unlike most other
casting techniques, centrifugal casting is chiefly used to
manufacture stock materials in standard sizes for further
In centrifugal casting, a permanent mold is rotated continuously
about its axis at high speeds (300 to 3000 rpm) as the molten metal
is poured. The molten metal is centrifugally thrown towards the
inside mold wall, where it solidifies after cooling. The casting is
usually a fine-grained casting with a very fine-grained outer
diameter, owing to chilling against the mould surface. Impurities and
inclusions are thrown to the surface of the inside diameter, which
can be machined away.
Casting machines may be either horizontal or verticalaxis. Horizontal axis machines are preferred for long, thin cylinders,
vertical machines for rings.
Features of centrifugal casting:
Castings can be made in almost any length, thickness & diameter.
Different wall thicknesses can be produced from the same size mold.
Eliminates the need for cores.
Resistant to atmospheric corrosion, a typical situation with pipes.
Mechanical properties of centrifugal castings are excellent
Only cylindrical shapes can be produced with this process.
Typical materials that can be cast with this process
are iron, steel, stainless steels, glass, and alloys
of aluminum, copper & nickel.
Two materials can be cast together by introducing a second
material during the process.
Typical parts made by this process are pipes, boilers, pressure
vessels ,flywheels, cylinder liners and other parts that are
axi-symmetric. It is notably used to cast cylinder
liners and sleeve valves for piston engines, parts which could
not be reliably manufactured otherwise.
1. On Basis of Size of Object to be Manufactured:
Size of cast objects vary over large range. An object from 5gm
to 200tonn, anything can be cast.
2. On Basis of Complexity:
Casting can be effectively used for complex shaped objects. It
can work where general machining processes can not be used,
as in complicated inner and outer shapes of object.
3. Weight Saving:
Component made with casting process is lighter than the
component made with other machining processes.
4. Control Over The Process:
Casting provides versatility. Wide range of properties can be
attained by adjusting percentage of alloying elements.
Casting can be made with hair like precision provided
proper molding and casting technique is employed.
6. Fibrous Structure:
Only casting have this advantage. Casting leaves
component with its solid fibrous structure which inherit
great compressive strength. So, component subjected to
compressive strength are made with casting eg IC engine
7. Control Over Grain Size:
Grain size of cast component can be easily controlled by
controlling cooling rate which in turn can be used to
modify the properties.
8. Low Cost:
Casing is one of cheapest method for mass production.
Though casting is cheapest for MASS Production, it
becomes non economical in case of JOB production.
Sand casting leaves rough surface which needs
machining in most of cases. It adds up the cost in
In sand casting, poor dimensional accuracy is achieved.
Cast products are superior for compressive loads but they
are very poor in tensile or shock loads.(They are brittle).